1 Structural Steel Pipe API Specification 2B Xth Edition, [Month][Year] API Monogram Program Effective Date: [Month][Day][Year]
2 1 Scope Structural Steel Pipe 1.1 Coverage This specification covers the fabrication of structural steel pipe formed from plate steel with longitudinal and circumferential butt-welded seams, typically in sizes 14 in. (355.6 mm) outside diameter and larger [40 in. (1.016 m) and larger for longitudinally welded double seam (LWDS)] with wall thickness 3 / 8 in. (9.5 mm) and greater (up to a nominal 40 ft length) suitable for use in construction of welded offshore structures. Also covered in this specification is high-frequency welded (HFW) pipe according to API 5L. The use of the electric resistance welded (ERW) process or spiral welded pipe is not included in this specification. Pipe fabricated under this specification is intended to be used primarily in piling and main structural members, including tubular truss connections, where internal stiffeners are not usually required. 1.2 Application of the API Monogram If the product is manufactured at a facility licensed by API and it is intended to be supplied bearing the API Monogram, the requirements of Annex A apply. 2 Normative References The following referenced documents are indispensable for the application of this document. For dated references, only the edition cited applies. For undated references, the latest edition of the referenced document (including any addenda) applies. API Specification 5L, Specification for Line Pipe AWS D , Structural Welding Code Steel 3 Definitions and Abbreviations 3.1 Definitions For the purpose of this specification, the following definitions apply can A section of structural steel pipe with no girth seam fabricator The person, firm, company, or corporation executing the contract or agreement with the purchaser to fabricate the structural steel pipe under this specification girth weld A circumferential butt-welded seam lying in a plane perpendicular to the longitudinal axis of the pipe, used to join tubular sections into lengths of straight pipe HFW pipe high-frequency welded pipe EW pipe produced with a welding current frequency equal to or greater than 70 khz longitudinal seam A butt-welded seam which parallels the axis of the pipe.
3 3.1.6 LWDS pipe longitudinally welded double seam pipe A can with two longitudinal seams, one of which may be made in the flat plate condition manufacturer The firm, company, or corporation furnishing plate steel used in the fabrication of the structural steel pipe mill pipe A structural steel pipe consisting of multiple cans joined by girth welds pile A cylindrical tubular member fabricated from one or more lengths of structural steel pipe, usually driven through a leg or sleeve of an offshore platform, that carries vertical loads and resists lateral forces pipe weld A longitudinal seam made after the plate has been formed into pipe plate weld A longitudinal seam made between flat plates which are subsequently formed into pipe purchaser The person, firm, company, or corporation entering into a contract or agreement for the purchase of structural steel pipe fabricated under this specification single seam welded pipe A can with one longitudinal seam, produced by a continuous welding process structural steel pipe A cylindrical tubular member formed from steel plate, having a uniform material and wall thickness, with longitudinal and/or circumferential butt welded seams, comprising of the following types: can, single seam welded pipe, longitudinally welded double seam (LWDS), and mill pipe. 3.2 Abbreviations CVN ERW HAZ HFW LWDS TMCP Charpy V-notch electric resistance welded heat affected zone high-frequency electric welding process for pipe during manufacturing longitudinally welded double seam thermo-mechanical control process
4 4 Material 4.1 Pipe furnished to this specification shall be fabricated from plate steel as specified by the purchaser. 4.2 The purchaser shall specify the grade and quality of plate steel to be used. When the plate steel is furnished by the fabricator, a mill test certificate shall be available and shall be furnished to the purchaser upon request. All plate shall bear mill identification numbers, including sections cut to size from the original mill-produced plate. Ultrasonic inspection, as a supplementary requirement to the designated plate specification, may be specified, if desired, when structural steel pipe is to be used in the fabrication of tubular joint cans in T, Y, and/or K connections where freedom from laminations and/or other internal defections is required. 4.3 For API 5L pipe intended to be used for structural purposes: a) The following requirements shall apply. 1) Specification: API 5L, PSL 2 2) Process of Manufacture: HFW 3) Delivery Condition: Thermo Mechanical Rolled or Formed (Condition M suffix to the grade), unless otherwise agreed 4) Plate ultrasonically inspected in accordance to the PSL 2 pipe ordered for offshore service requirements of API 5L 5) Jointers not be furnished 6) The WPS & PQR in accordance with the manufacturing procedure qualification for PSL 2 pipe requirements of API 5L provided upon request 7) NDT system capability records provided upon request and are to be in accordance with the nondestructive inspection for other than sour service or offshore service requirements of API 5L 8) Both ends of each length marked on the OD of the pipe in accordance with API 5L and covered by mill varnish 9) The out-of-roundness (ovality) at any point in the pipe length not exceed 1.0 % of the specified diameter, in accordance with this specification 10) Unless otherwise specified on the purchase agreement, the maximum allowable straightness deviation not exceed 0.15 % of the pipe length b) The purchase agreement shall include the following information. 1) API 5L, PSL 2 HFW pipe for use with welded connectors 2) Order quantity for each item 3) Specified outside diameter, wall thickness, and grade 4) Length and length tolerance
5 c) The purchase agreement shall also state which of the following provisions are applicable for the specific order item. 1) If other than Thermo Mechanical Rolled or Formed (Condition M suffix to the grade), Delivery Condition as specified on the purchase agreement 2) API 5L, weldability of PSL 2 pipe requirements 3) OD grinding of the weld cap for a minimum distance of 4 ft (1.22 m) from one end and 10 ft (3.05 m) from the other. The dimensional tolerance shall be + 1 / 16, -0.0 in. (+1.6, -0.0 mm) for the weld bead height and retention of the minimum wall thickness [at no point shall the weld bead after grinding be below the surface of the pipe nor shall it be raised above the parent metal by more than 1 / 16 in.(1.6 mm)]. 4) Full length OD mill varnish in accordance with API 5L 5) Pipe shall be ID drift tested full-length at a frequency of 10 %, unless otherwise specified in the purchase agreement. Unless otherwise specified, the drift mandrel dimensions shall be 98 % of the calculated ID, 24 in. (609.6 mm) in length, and a notch for the weld cap is not allowed. 6) Longitudinal and/or transverse tensile tests before and after simulated post weld heat treat conditions at a minimum frequency of one test per order, unless otherwise specified, for each combination of diameter, wall thickness, and grade for each supplier chemistry type and mill process. The purchaser shall also specify the heat treat cycle time and temperature, and acceptance criteria. 7) Application of the API Monogram marking in accordance with API 5L. 5 Fabrication 5.1 General Forming pipe furnished to this specification shall normally be formed below 400 F (204 C) that is, cold formed. Warm forming [between 800 F and 1200 F or 50 F (427 C and 649 C or 10 C) below the tempering temperature of quenched and tempered steels] may be employed provided forming procedures for heat treated or TMCP steel are qualified to demonstrate the mechanical strength properties required by the original plate specification are met in the warm formed condition. Hot forming (above the upper critical temperature) may also be employed provided the forming procedure is qualified to demonstrate all mechanical properties required by the original plate specifications are met The purchaser may specify Supplementary Requirement 1 (SR1) from Annex B if the rolled direction of the plate is desired to be oriented in a specific direction during the forming of the pipe, and the pipe shall be so identified All welding shall be in accordance with AWS D Unless otherwise approved by the purchaser, the submerged arc welding process shall be employed for all welding except tack welds, root passes, and repair welding where other AWS approved processes may be utilized. All welds shall be complete joint penetration groove welds produced by employing AWS D prequalified joint details, or other joint configurations qualified by procedure qualification testing. Welding electrodes and fluxes shall conform to applicable AWS specifications and shall be selected to match the minimum ultimate strength of the base material, and to provide a minimum of 20 ft-lbs (28 J) Charpy V-notch (CVN) impact energy at 0 F ( 8 C). Matching CVN toughness may be specified by invoking Supplementary Requirement 4 (SR4) in Annex B.
6 If the AWS specification requirement for the electrodes and fluxes to be employed is less than the foregoing, or if the welding procedure falls outside the range of essential variables tested in the AWS specification, then Charpy test specimens shall be removed from a simulated production weld and tested in accordance with Annex III of AWS D The deposited weld metal shall possess an energy value not less than indicated. The foregoing requirements shall apply separately to the final condition of plate welds, pipe welds, and girth welds. All welding shall conform to the minimum workmanship standards of Section 5 of AWS D Welding Procedure Qualification The welding procedures shall be established in accordance with AWS D Written prequalified welding procedures may be employed by the fabricator provided the procedure complies with all requirements (joint detail, filler metal, and so forth) for prequalified status detailed in Appendix IV of AWS D More stringent Charpy V-notch toughness in the weld and/or heat affected zones than required in above may be obtained, if desired, by specification of Supplementary Requirement 2 (SR2) in Annex B. The welding procedures shall be established in accordance with AWS D Written prequalified welding procedures may be employed by the fabricator provided the procedure complies with all requirements (joint detail, filler metal, etc.) for prequalified status detailed in Appendix IV of AWS D More stringent CVN toughness in the weld and/or heat affected zones than required in 3.3 may be obtained, if desired, by specification of SR2. The foregoing requirements shall apply separately to plate welds, pipe welds, and girth welds. 5.3 Welder and Welding Operator Qualification Welders and welding operators shall be qualified in accordance with AWS D , Chapter 4, Part B or C, as applicable. Radiography is acceptable for the qualification of submerged arc machine operators. 5.4 Longitudinal Welds Radial offset of abutting edges of longitudinal weld seams shall not exceed 1 / 8 in. (3.2 mm). For LWDS pipe, no two longitudinal seams shall be closer together than one pipe diameter or 5 ft (1.524 m), whichever is greater. Longitudinal weld seams of adjoining cans shall be staggered as shown in Table 1 below, unless closer spacing is agreed upon by the purchaser and the fabricator. Table 1 Seam Spacing and Stagger Seam Spacing Stagger 360 (single seam) (LWDS) other (LWDS) min 25 % of smaller seam spacing 5.5 Girth Welds Radial offset of abutting edges of the girth seams shall not exceed 0.2T (where T is the wall thickness) or 1 / 4 in. (6.4 mm) maximum provided the offset exceeding 1 / 8 in. (3.2 mm) is welded from both sides. One localized area per girth weld up to 0.3T, or 3 / 8 in. (9.5 mm) maximum, is permitted provided the localized area is under 8T in length and weld metal is added to this region to provide a 4:1 tapered transition. No two girth welds shall be located closer together than one pipe diameter or 3 ft (0.914 m), whichever is less. There shall be no more than two girth welds in any 10 ft (3.05) interval of pipe. For LWDS pipe, no two girth welds shall be located closer together than 10 ft (3.05 m). This requirement does not apply to subsequent fabrication which incorporates the mill pipe into a pile or structure.
7 6 Dimensions and Tolerances 6.1 Diameter, Length, and Wall Thickness The diameter, length, and wall thickness of pipe furnished to this specification shall be as specified by the purchaser. The length of each pipe shall not vary from the specified nominal length more than ±1-1 / 2 in. (38.1 mm) per 10 ft (3.05 m) of length. For conversion to metric units, see Annex C. 6.2 Roundness The out-of-roundness, that is, the difference between the major and minor outside diameters at any point in a length of pipe, shall not exceed 1 % of the nominal diameter or 1 / 4 in. (6.4 mm) maximum for wall thicknesses up to and including 2 in. (50.8 mm). For wall thickness exceeding 2 in. (50.8 mm), the maximum permitted deviation shall not exceed an out-of-roundness to wall thickness ratio of 1:8. For pipe exceeding 48 in. (1.22 m) diameter, a maximum deviation of 1 / 2 in. (12.7 mm) shall be permitted provided the circumference tolerance is maintained within ± 1 / 4 in. (6.4 mm). 6.3 Circumference The outside circumference at any point in a length of pipe shall be within ±1 % of the nominal circumference or within ± 1 / 2 in. (12.7 mm), whichever is less. 6.4 Straightness The maximum allowable straightness deviation in any 10 ft (3.05 m) length shall be 1 / 8 in. (3.2 mm). For lengths over 10 ft (3.05 m), the maximum deviation of the entire length may be computed by the following formula, not to exceed 3 / 8 in. (9.5 mm) in any 40 ft (12.19 m) length. 1 total length (in.) in. * 8 10ft (1) 6.5 Pipe Ends Unless otherwise specified, all pipe shall be beveled for welding with an angle of 30 ±2.5 (measured from a line perpendicular to the surface of the pipe) with a root face of 1 / 16 in. (1.6 mm) ± 1 / 32 in. (0.8 mm). The root face shall be perpendicular to the longitudinal axis of the pipe within 1 / 16 in. per ft of diameter, with a maximum allowable deviation of 1 / 4 in. (6.4 mm), measured with a square and straight edge across the end of the pipe. 7 Inspection and Repair 7.1 Inspection Fabrication and verification inspection shall be conducted in accordance with the requirements of AWS D , Section 6, to assure compliance with the applicable requirements of Sections 1 through Weld Inspection All welds shall be visually inspected on both the inside and outside surfaces. The weld profile shall meet the requirements of AWS D , Section Nondestructive Examination 100 % of each girth weld and spot testing amounting to 10 % of each longitudinal weld (including the extreme ends) shall be examined by radiographic or ultrasonic inspection in accordance with the requirements of Section 6 and Part E with Paragraph and Part F with Paragraph of AWS D More extensive radiographic coverage may be obtained, if desired, by specification of Supplementary Requirement 3 (SR3) in Annex B. The fabricator shall be responsible for conducting all radiographic examinations.
8 7.4 Repair of Base Metal Imperfections Imperfections detected in the base metal shall be explored to determine the extent of each. Imperfections in the finished tube no deeper than 5 % of the specified nominal wall thickness and mechanical marks no deeper than 5 % of the nominal wall thickness or 1 / 16 in. (1.6 mm) in depth need not be removed. Imperfections which exceed the above shall be ground to sound metal. The excavation area shall be faired, and the thickness in the ground area shall not be reduced more than 7 % of the nominal thickness but in no case more than 1 / 8 in. (3.2 mm) depth. If the depth of imperfections in as-rolled plate exceeds the above limits, but not more than 20 % of the nominal thickness, welding repairs may be performed. Repair of defects deeper than 20 % of the nominal wall thickness or repair of defects with a length and/or width more than 20 % of the nominal diameter shall not be permitted. Tubulars made from other than asrolled plate shall not be repaired by welding unless specifically approved by the purchaser. 8 Marking Pipe fabricated in conformance with this specification shall be marked by an API licensed fabricator as specified below. Each section of the pipe shall be paint stenciled on the inside of both ends in letters a minimum of 1 in. high with the following. a) fabricator s name b) API Monogram c) API 2B d) other industry standard (e.g. API 5L, ASTM standard, etc.) of steel plate e) nominal outside diameter f) nominal wall thickness g) specified supplementary requirements (i.e. SR1, SR2, SR3 and/or SR4 in Annex B) 9 Suggestions for Ordering API 2B Pipe 9.1 In placing orders for steel pipe to be fabricated in accordance with this specification, the purchaser should specify the following on the purchase order: Specification..API 2B Quantity Size. as required Other industry standard (e.g. ASTM) for steel plate...nominal length, wall thickness, and OD Delivery date and shipping instructions...as required 9.2 In placing orders for steel pipe to be fabricated in accordance with this specification, the purchaser should state whether any of the following optional or supplementary requirements are to apply: Mill test certificate for steel plate End finish (specify, in not standard 30 bevel) SR1 plate direction of rolling Longitudinal S-1L Transverse S-1T SR2 notch toughness (specify test temperatures and minimum energy requirements) SR3 100 % radiographic examination (joint can quality assurance) SR4 matching weld toughness for designated plate material
9 Annex A (informative) A.1 Scope A.1.1 Applicability API Monogram Program Use of the API Monogram by Licensees This annex is normative (mandatory) for products supplied bearing the API Monogram and manufactured at a facility licensed by API; for all other instances it is not applicable. A.1.2 General The API Monogram is a registered certification mark owned by the American Petroleum Institute (API) and authorized for licensing by the API Board of Directors. Through the API Monogram Program, API licenses product manufacturers to apply the API Monogram to products which comply with product specifications and have been manufactured under a quality management system that meets the requirements of API Q1. API maintains a complete, searchable list of all Monogram licensees on the API Composite List website ( The application of the API Monogram and license number on products constitutes a representation and warranty by the licensee to API and to purchasers of the products that, as of the date indicated, the products were manufactured under a quality management system conforming to the requirements of API Q1 and that the product conforms in every detail with the applicable standard(s) or product specification(s). API Monogram program licenses are issued only after an on-site audit has verified that an organization has implemented and continually maintained a quality management system that meets the requirements of API Q1 and that the resulting products satisfy the requirements of the applicable API product specification(s) and/or standard(s). Although any manufacturer may claim that its products meet API product requirements without monogramming them, only manufacturers with a license from API can apply the API Monogram to their products. Together with the requirements of the API Monogram license agreement, this annex establishes the requirements for those organizations who wish to voluntarily obtain an API license to provide API monogrammed products that satisfy the requirements of the applicable API product specification(s) and/or standard(s) and API Monogram Program requirements. For information on becoming an API Monogram Licensee, please contact API, Certification Programs, 1220 L Street, NW, Washington, DC or call (202) or by at A.2 Normative References In addition to the referenced standards listed earlier in this document, this annex references the following standard: API Specification Q1, Specification for Quality Management System Requirements for Manufacturing Organizations for the Petroleum and Natural Gas Industry For Licensees under the Monogram Program, the latest version of this document shall be used. The requirements identified therein are mandatory.
10 A.3 API Monogram Program: Licensee Responsibilities A.3.1 Monogram Program Requirements For all organizations desiring to acquire and maintain a license to use the API Monogram, conformance with the following shall be required at all times: a) quality management system requirements of API Q1; b) API Monogram Program requirements of API Q1, Annex A; c) requirements contained in the API product specification(s) to which the organization is licensed; and d) requirements contained in the API Monogram Program License Agreement. A.3.2 Control of the Application and Removal of the API Monogram Each licensee shall control the application and removal of the API Monogram in accordance with the following: a) products that do not conform to API specified requirements shall not bear the API Monogram; b) each licensee shall develop and maintain an API Monogram marking procedure that documents the marking/monogramming requirements specified by this annex and any applicable API product specification(s) and/or standard(s). The marking procedure shall: 1) define the authority responsible for application and removal of the API Monogram and license number; 2) define the method(s) used to apply the Monogram and license number; 3) identify the location on the product where the API Monogram and license number are to be applied; 4) require the application of the date of manufacture of the product in conjunction with the use of the API Monogram and license number; 5) require that the date of manufacture, at a minimum, be two digits representing the month and two digits representing the year (e.g for May 2012) unless otherwise stipulated in the applicable API product specification(s) or standard(s); and 6) define the application of all other required API product specification(s) and/or standard(s) marking requirements. c) only an API licensee shall apply the API Monogram and its designated license number to API monogrammable products; d) the API Monogram and license number, when issued, are site-specific and subsequently the API Monogram shall only be applied at that site specific licensed facility location; and e) the API Monogram may be applied at any time appropriate during the production process but shall be removed in accordance with the licensee s API Monogram marking procedure if the product is subsequently found to be out of conformance with any of the requirements of the applicable API product specification(s) and/or standard(s) and API Monogram Program.
11 For certain manufacturing processes or types of products, alternative API Monogram marking procedures may be acceptable. Requirements for alternative API Monogram marking are detailed in the, API Monogram Program Alternative Marking of Products License Agreement, available on the API Monogram Program website at A.3.3 Design and Design Documentation Each licensee and/or applicant for licensing shall maintain current design documentation as identified in API Q1 for all of the applicable products that fall under the scope of each Monogram license. The design document information shall provide objective evidence that the product design meets the requirements of the applicable and most current API product specification(s) and/or standard(s). The design documentation shall be made available during API audits of the facility. In specific instances, the exclusion of design activities is allowed under the Monogram Program, as detailed in Advisory #6, available on API Monogram Program website at A.3.4 Manufacturing Capability The API Monogram Program is designed to identify facilities that have demonstrated the ability to manufacture equipment that conforms to API specifications and/or standards. API may refuse initial licensing or suspend current licensing based on a facility s level of manufacturing capability. If API determines that an additional review is warranted, API may perform additional audits (at the organization s expense) of any subcontractors to ensure their conformance with the requirements of the applicable API product specification(s) and/or standard(s). A.3.5 Use of the API Monogram in Advertising An API Monogram licensee shall not use the API Monogram and/or license number on letterheads, buildings or other structures, websites or in any advertising without an express statement of fact describing the scope of Licensee s authorization (license number and product specification). The Licensee should contact API for guidance on the use of the API Monogram other than on products. A.4 Product Marking Requirements A.4.1 General These marking requirements shall apply only to those API Licensees wishing to mark applicable products in conjunction with the requirements of the API Monogram Program. A.4.2 Product Specification Identification Manufacturers shall mark products as specified by the applicable API specifications or standards. Marking shall include reference to the applicable API specification and/or standard. Unless otherwise specified, reference to the API specifications and/or standards shall be, as a minimum, API [Document Number] (e.g. API 6A or API 600). Unless otherwise specified, when space allows, the marking may include use of Spec or Std, as applicable (e.g. API Spec 6A or API Std 600). A.4.3 Units Products shall be marked with units as specified in the API specification and/or standard. If not specified, equipment shall be marked with U.S. customary (USC) units. Use of dual units [USC units and metric (SI) units] may be acceptable, if such units are allowed by the applicable product specification and/or standard.
12 A.4.4 Nameplates Nameplates, when applicable, shall be made of a corrosion-resistant material unless otherwise specified by the API specification and/or standard. Nameplate shall be located as specified by the API specification and/or standard. If the location is not specified, then the licensee shall develop and maintain a procedure detailing the location to which the nameplate shall be applied. Nameplates may be attached at any time during the manufacturing process. The API Monogram and license number shall be marked on the nameplate, in addition to the other product marking requirements specified by the applicable product specification and/or standard. A.4.5 License Number The API Monogram license number shall not be used unless it is marked in conjunction with the API Monogram. The license number shall be used in close proximity to the API Monogram. A.5 API Monogram Program: Nonconformance Reporting API solicits information on products that are found to be nonconforming with API specified requirements, as well as field failures (or malfunctions), which are judged to be caused by either specification and/or standard deficiencies or nonconformities against API specified requirements. Customers are requested to report to API all problems with API monogrammed products. A nonconformance may be reported using the API Nonconformance Reporting System available at
13 Annex AB (informative) B.1 General Supplementary Requirements When specified on the purchase order, the following supplementary requirements shall apply (i.e. SR1, SR2, SR3, and/or SR4). B.2 SR1 Plate Rolling Direction Orientation B.2.1 The orientation of the pipe axis relative to the final rolling direction of the plate from which the pipe is formed shall be longitudinal or transverse (circumferential) as indicated on the purchase order and illustrated below. B.2.2 Pipe fabricated in accordance with this supplementary requirement shall be identified by marking S-lL or S-lT adjacent to API 2B as required by Section 8, items e and g. See Figure AB.1.
14 B.3 SR2 CVN Toughness Tests Notch toughness tests shall be conducted as a requirement of the welding procedure qualification tests. The welding procedure qualification test coupon shall be welded and tested in accordance with Paragraph of AWS D Charpy V-notch test specimens shall be removed from the weld and heat affected zone in accordance with the requirements of Appendix III of AWS D The test temperature, notch location (if different from AWS), and the minimum average energy value shall be as indicated on the purchase order. The pipe shall be identified by marking as required in Section 8, item g. B.4 SR3 100 Percent Radiographic Examination In addition to 100 % radiography of the girth welds specified by 7.3, each designated longitudinal weld shall be examined by radiography throughout its entire length. Pipe inspected in accordance with this supplementary requirement shall be identified by marking as required in Section 8, Item g. B.5 SR4 Matching Weld CVN Toughness for Designated Plate Material B.5.1 Depending on the Strength Group and Toughness Class of the designated API or ASTM plate specification, as given in Table C2.4 of AWS D , the corresponding required weld metal CVN toughness shall be as given in Table C4.1 of AWS D , and the heat affected zone (HAZ) CVN toughness shall be given in Table C4.2 of AWS D B.5.2 Charpy test specimens shall be removed from both the weld metal and HAZ of a simulated production weld and tested in accordance with Annex III of AWS D The deposited weld metal and HAZ shall possess average energy values not less than indicated in Tables C4.1 and C4.2 of AWS D , respectively, and no single test shall be more than 5 ft-lbs (7 J) lower. The foregoing requirements shall apply separately to plate welds, pipe welds and girth welds. B.5.3 For steels not listed in Table C2.4 of AWS D , or in Table B.1 below, the purchaser shall designate the group and class for which matching weld toughness is desired. HAZ requirements for Group III, Class B shall be the same as for Group II, Class B. Table B.1 Additional Steel Requirements Additional Steel Group Class API 2MT1 II B B.5.4 Further guidance is given in Sections C and C of AWS D
15 Annex BC (informative) Metric Conversion Table Application of the following equivalent values may be employed when converting the units of measure employed herein to standard metric (SI) practice. Table BC.1 Metric Conversion Table Stated Value Metric Value 1 / 32 in. 0.8 mm / 16 in. 1.6 mm / 8 in. 3.2 mm / 4 in. 6.4 mm / 8 in. 9.5 mm / 2 in mm 1-1 / 2 in mm 2 in mm 48 in m 10 ft 3.05 m 40 ft m 0 F -18 C 50 F 10 C 400 F 204 C 800 F 427 C 1200 F 649 C 20 ft-lbs 28 J
16 Bibliography  API Specification 2MT1, Rolled Shapes with Improved Notch Toughness  ASTM A6-99, General Requirements for Rolled Steel Plates, Shapes, Sheet Piling, and Bars for Structural Use  ASTM A20-99, General Requirements for Delivery of Steel Plates for Pressure Vessels  ASTM A370-97, Mechanical Testing of Steel Products  ASTM E23-98, Notched Bar Impact Testing of Metallic Materials